Synergy between Spin Crossover and Metallophilicity in Triple Interpenetrated 3D Nets with the NbO Structure Type
Ana Galet; Virginie Niel; M. Carmen Muñoz; José A. Real; Journal of the American Chemical Society 125 (2003) 14224–14225; doi:10.1021/ja0377347

data_4114408
_publ_section_title
;
 Synergy between Spin Crossover and Metallophilicity in Triple
 Interpenetrated 3D Nets with the NbO Structure Type
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              14224
_journal_page_last               14225
_journal_paper_doi               10.1021/ja0377347
_journal_volume                  125
_journal_year                    2003
_chemical_formula_sum            'C48 H28 Ag6 Fe3 N24 O2'
_chemical_formula_weight         1787.71
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           147
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3'
_symmetry_space_group_name_H-M   'P -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   15.2900(9)
_cell_length_b                   15.2900(9)
_cell_length_c                   6.9050(3)
_cell_measurement_temperature    145(2)
_cell_volume                     1398.01(13)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      145(2)
_diffrn_measured_fraction_theta_full 0.972
_diffrn_measured_fraction_theta_max 0.972
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0336
_diffrn_reflns_av_sigmaI/netI    0.0696
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            3473
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_diffrn_reflns_theta_min         4.07
_exptl_absorpt_coefficient_mu    2.871
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.123
_exptl_crystal_description       parallelepipeds
_exptl_crystal_F_000             860
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.06
_refine_diff_density_max         0.655
_refine_diff_density_min         -0.616
_refine_diff_density_rms         0.115
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.961
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     95
_refine_ls_number_reflns         2077
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.961
_refine_ls_R_factor_all          0.0637
_refine_ls_R_factor_gt           0.0333
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0266P)^2^+0.3924P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0629
_refine_ls_wR_factor_ref         0.0693
_reflns_number_gt                1504
_reflns_number_total             2077
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja0377347si20031016_123855.cif
_cod_data_source_block           global
_cod_database_code               4114408